Presentation on theme: "Amendments to the Specifications Discussion of Changes to the Concrete Materials Specifications."— Presentation transcript:
Amendments to the Specifications Discussion of Changes to the Concrete Materials Specifications
What is in your handout? Version of Section 90, “Portland Cement Concrete” of the Standard Specifications highlighting all changes made in 2009 (portion of S1-020) Versions of SSPs S8-C04 and S8-C05 highlighting changes made in 2009 All new SSP S8-C02 created in 2009
page 1: Class Concrete No longer designating concrete by "Class", but by minimum cementitious material content and minimum strength. Why?
page 2: Compressive Strength Default Compressive Strength = 2500 psi Except for when a modulus of rupture is specified, the minimum required compressive strength for concrete shall be the strength specified, or 2,500 pounds per square inch, whichever is greater. Concrete shall be proportioned such that the concrete will attain the minimum required compressive strength. For concrete not designated by compressive strength, the Engineer may test the concrete for compressive strength. The concrete will be accepted if the compressive strength at 28 days attains 85 percent or more of the minimum required compressive strength.
Intergrinding Limestone ASTM C150 Conclusion: Cements tested with limestone had better short-term strength and less permeability, but slightly higher shrinkage (at 90 days). Accept the full 5 percent specified by ASTM C 150 but add shrinkage control. Caltrans recently finished a study to evaluate the effect of limestone on concrete performance.
page 4 (con’t) : The List No cementitious material shall be used in the work unless it is on the Department's Pre- Qualified Products List at the time of mix design submittal. Information regarding cementitious material qualification and placement on the Department's approved list can be obtained at the Transportation Laboratory.
page 5 : Blended Cement Blended cement shall conform to the requirements for Portland Blast-Furnace Slag Cement, Type IS (MS) or Portland-Pozzolan Cement, Type IP (MS) in AASHTO Designation: M 240, except that the maximum limits on the pozzolan content shall not apply. Blended cement shall be comprised of Type II or Type V cement and SCM produced either by intergrinding portland cement clinker and SCM, by blending portland cement and either finely ground granulated blast furnace slag or finely divided pozzolan, or a combination of intergrinding and blending.
page 5 (con’t) : Silos and COC’s Facilities shall be provided to ensure that the various cementitious materials meeting this Section 90 ‑ 2.01 are kept separate from each other and from other cementitious materials. A storage silo containing a cementitous material shall be emptied before using that silo for a different cementitious material. Blended cements with a percentage of SCM differing by more than 2 percentage points are considered different cementitious materials. Sampling cementitious materials shall be in conformance with California Test 125. If blended cement is used, the Certificate of Compliance shall include a statement signed by the blended cement supplier that indicates the actual percentage, by weight, of SCM in the blend. Weight of SCM shall be by weighing device conforming to Section 9-1.01, "Measurement of Quantities," or as determined by chemical analysis.
pages 10 & 11 : Precast Options B.Fly Ash + LiNO 3 C.ASTM C 1567 (0.10% expansion) A.
page 12 : Innocuous Aggregate To be considered "innocuous," aggregate must be on the Department's approved list, "Innocuous Aggregates for use in Concrete." Information regarding aggregate qualification and placement on the Department's approved list can be obtained at the Transportation Laboratory. Both coarse and fine aggregate must be on the approved list for the aggregate used in concrete to be considered innocuous. A.ASTM C 1293 >> 1 year >> 0.04% expansion or B.ASTM C 1260 >> 16 days >> 0.15% expansion
Innocuous Aggregate…? For Precast Concrete (Equation 3): For Cast-In-Place Concrete (Equation 1):
pages 14 & 17 : Admixtures C. Lithium Nitrate shall be in an aqueous solution conforming to the following: 1. Lithium Nitrate (LiNO3) must be 30% +/- 0.5% by weight 2. Sulfate (SO4) must be less than 1000 ppm 3. Chloride (Cl) must be less than 1000 ppm 4. Alkalis (Na2O + 0.658 K2O) must be less than 1000 ppm The Contractor may use a Type S admixtures conforming to the requirements in ASTM Designation: C 494. SRAs VMAs Lithium Nitrate
page 21 : Mixing Water No additional mixing water shall be incorporated into the concrete during hauling or after arrival at the delivery point. unless authorized by the Engineer. If the Engineer authorizes additional water to be incorporated into the concrete, the drum shall be revolved not less than 30 revolutions at mixing speed after the water is added and before discharge is commenced.
page 29 : Minor Concrete Before using minor concrete or in advance of revising the mix proportions, the Contractor shall submit in writing to the Engineer a copy of the mix design. When required by the following table, the Contractor shall include compressive strength test results verifying the minimum specified compressive strength: SCMTest Submittal Required Fly Ash used aloneWhen portland cement content<350 lbs/cy GGBFS used aloneWhen portland cement content <250 lbs/cy Natural Pozzolan used alone When portland cement content <350 lbs/cy More than 1 SCMAlways Tests shall be performed by an ACI certified technician. Cementitious material shall conform to the provisions in Section 90 ‑ 1.01, "Description,." and 90-2, "Materials."
page 32 : Strength Development Time (S8- C02) The time allowed to obtain the minimum required compressive strength as specified in Section 90-1.01, "Description," of the Standard Specifications will be 56 days when the Contractor chooses cementitious material that satisfies the following equation: (41 x UF) + (19 x F) + (11 x SL) 7.0 TC ALLOW 56 days
page 33 : Rice Hull Ash (S8-C02) The Contractor may use rice hull ash as a supplementary cementitious material (SCM) to make minor concrete. Rice hull ash shall conform to the requirements in AASHTO Designation: M 321 and the following chemical and physical requirements: Only for
page 34 : Corrosion Control (S8- C04) An exception to the equations in Section 90-2.01C chlorides sulfates pH Use one of These options and call me in the morning When?
pages 37, 38, & 39 : Freezing Conditions (S8-C05) 2 parts to this SSP: 1.“Concrete Near Deicing Chemicals” 2.“Cementitious Material” (all other concrete in this environment)
What does Caltrans get from these revisions? Stronger Longer Lasting More Dense More Durable Better ASR Protection More Corrosion Resistant Sustainable Cheaper Greener (x2)